View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
1.
CHAPTER
1
Fundamentals of
Extrusion
The first chapter of this book discusses the fundamentals of extrusion
technology, including extrusion principles, processes, mechanics, and
variables and their effects on extrusion. The extrusion industry is now
over 100 years old. A concern within the industry is the continuing education necessary to upgrade knowledge about aluminum extrusion technology, both in the academic and industrial communities.
In a typical university manufacturing engineering and technology
course, textbooks, such as Ref 1, normally used in engineering schools
across the world cover the principles and very fundamental aspects of
manufacturing processes, including metal cutting, rolling, forging,
drawing, and extrusion. Engineers and product designers are not specifically taught about the extrusion process in detail in either their university or job training. Surely, proper education is essential for success in
the field of aluminum extrusion technology. It is necessary for technical
and engineering personnel to be familiar with the fundamental concepts. Once the basics are understood, additional levels of sophistication can be gradually added.
Definition of Extrusion
Extrusion is a plastic deformation process in which a block of metal
(billet) is forced to flow by compression through the die opening of a
smaller cross-sectional area than that of the original billet as shown in
Fig. 1. Extrusion is an indirect-compression process. Indirect-compressive
2.
2 / Aluminum Extrusion Technology
Fig. 1
Definition and principle of extrusion
forces are developed by the reaction of the workpiece (billet) with the
container and die; these forces reach high values. The reaction of the
billet with the container and die results in high compressive stresses that
are effective in reducing the cracking of the billet material during primary breakdown from the billet (Ref 2). Extrusion is the best method
for breaking down the cast structure of the billet because the billet is
subjected to compressive forces only.
Extrusion can be cold or hot, depending on the alloy and the method
used. In hot extrusion, the billet is preheated to facilitate plastic deformation.
Classification of Extrusion Processes
The two basic types of extrusion are direct and indirect, which are
commonly used in aluminum industries as shown in Fig. 1 and 6. Solid
and hollow shapes are designed and extruded for a wide range of programs:
•
•
•
•
•
Solid sections, bars, and rods extruded from solid billets by direct
extrusion (discussed in Chapter 3)
Tubes and hollow sections extruded from solid billets through porthole or bridge-type dies (for certain alloys) by direct extrusion (discussed in Chapter 6)
Tubes and hollow sections extruded from hollow or solid billets
(latter pierced in the press via floating mandrel) by direct extrusion
(discussed in Chapter 3)
Tubes and hollow sections extruded from hollow or solid billets
(latter pierced in the press via stationary mandrel) by direct extrusion
Critical solid sections, bars, and rods extruded from solid billets
with sealed container through the die mounted on the stem by indirect extrusion (discussed in Chapter 3)
3.
Fundamentals of Extrusion / 3
•
Tubes and hollow sections extruded from hollow or solid billets
(latter pierced in press) via stationary mandrel through the die
mounted on the stem by the indirect extrusion process
Conventional Direct Extrusion
The most important and common method used in aluminum extrusion
is the direct process. Figure 1 shows the principle of direct extrusion
where the billet is placed in the container and pushed through the die by
the ram pressure. Direct extrusion finds application in the manufacture
of solid rods, bars, hollow tubes, and hollow and solid sections according to the design and shape of the die. In direct extrusion, the direction
of metal flow will be in the same direction as ram travel. During this
process, the billet slides relative to the walls of the container. The resulting frictional force increases the ram pressure considerably. During
direct extrusion, the load or pressure-displacement curve most commonly has the form shown in Fig. 2. Traditionally, the process has been
described as having three distinct regions:
1. The billet is upset, and pressure rises rapidly to its peak value.
2. The pressure decreases, and what is termed “steady state” extrusion
proceeds.
3. The pressure reaches its minimum value followed by a sharp rise as
the “discard” is compacted.
Billet-on-Billet Extrusion
Billet-on-billet extrusion is a special method for aluminum alloys that
are easily welded together at the extrusion temperature and pressure.
Using this process, continuous lengths of a given geometry (shape) can
be produced by different methods. Billet-on-billet extrusion is also a viable process in the production of coiled semifinished products for further
Fig. 2
Variation of load or pressure with ram travel for both direct and indirect extrusion process
4.
4 / Aluminum Extrusion Technology
processing, such as rod and tube drawing production. Perfect welding
of the billet in the container with the following billet must take place as
the joint passes through the deformation zone. The following requirements have to be fulfilled (Ref 3):
•
•
•
•
•
Good weldability at the temperature of deformation
Accurate temperature control
Cleaned billet surface
Sawn, clean billet ends free from grease
Bleeding of air from the container at the start of the extrusion using
taper-heated billet as shown in Fig. 3 to avoid blisters and other defects
Two methods of billet-on-billet extrusion have been developed. In the
first method, the discard is removed, and the following billet is welded
to the one remaining in the welding or feeder plate (Fig. 4).
Fig. 3
Bleeding out air during upsetting
Fig. 4
Continuous-type extrusion using welding plate in front of the die
(method 1)
5.
Fundamentals of Extrusion / 5
The second method does not need a discard; the subsequent billet is
pressed directly onto the billet still in the container as shown in Fig. 5.
The dummy block attached with the stem shears an aluminum ring from
the container during each return stroke, and this has to be removed from
the stem (Ref 3).
Indirect Extrusion
In indirect extrusion, the die at the front end of the hollow stem moves
relative to the container, but there is no relative displacement between
the billet and the container as shown in Fig. 6. Therefore, this process is
characterized by the absence of friction between the billet surface and
the container, and there is no displacement of the billet center relative to
the peripheral regions. The variation of load or pressure with the ram
travel during both direct and indirect extrusion processes is shown in
Fig. 2.
Fig. 5
Billet-on-billet extrusion (method 2)
Fig. 6
Indirect extrusion process
6.
6 / Aluminum Extrusion Technology
Mechanics of Extrusion
Plastic Deformation and Metal Flow
In metal forming, plasticity theory is applied to investigate the mechanics of plastic deformation. The investigation allows the analysis
and prediction of the following:
•
•
•
•
Metal flow, including velocities, strain rates, and strain
Temperature and heat transfer
Variation of local material strength or flow stress of material
Stresses, forming load, pressure, and energy
The mechanics of plastic deformation provide the means for determining how the metal flows in different forming operations, the means
of obtaining desired geometry through plastic deformation, and the
means for determining the expected mechanical and physical properties
of the metal produced. Different mathematical equations can be obtained through a different approach (Ref 4 to 7) for different forming
operations, including extrusion.
In simple homogeneous (uniaxial) compression or in tension, the
metal flows plastically when the stress, σ, reaches the value of flow
stress, σ. The flow of aluminum during extrusion is intermetallic shear
flow. The significant difference in the shear flow of aluminum compared with other metals being extruded is that the center of the aluminum billet is extruded first, and the peripheral part of the billet flows
later, causing more severe shear deformation. As soon as the force required to push the billet into the container surface exceeds that of the
shear strength of the billet material, sticking friction predominates, and
deformation proceeds by shear in the bulk of the billet. Metal flow during extrusion depends on many factors, such as the following:
•
•
•
Billet material property at billet temperature
Billet-container interface and metal-die interface friction
Extrusion ratio
A fairly large number of investigations of the flow characteristics of
metal, such as lead, tin, and aluminum, have been made by using a
split-billet technique (Ref 3 and 7 to 9). Typical flow patterns observed
in extrusion are shown in Fig. 7 (Ref 3).
In extrusion of homogeneous materials, flow pattern S is found in the
absence of friction at the container and die interfaces. The extrusion
properties should be uniform in both longitudinal and transverse directions,
respectively. This flow pattern is usually obtained in fully lubricated
conditions in both container and dies.
7.
Fundamentals of Extrusion / 7
Fig. 7
Schematic of the four different types of flow in extrusion. Source: Ref 3
Flow pattern A is obtained in extrusion of homogeneous materials in
the presence of friction at the die interface, not at the container-billet interface. This flow pattern is good for indirect extrusion. The metal at the
center of the billet moves faster than the metal at the periphery. In the
corner of the leading end of the billet, a separate metal zone is formed
between the die face and the container wall, known as a dead-metal
zone. The material near the surface undergoes shear deformation compared with the pure deformation at the center, and it flows diagonally
into the die opening to form the outer shell of extrusion.
Flow pattern B is obtained in homogeneous materials when there is
friction in both container and die interfaces. This flow pattern is good
for direct extrusion processes. An extended dead-metal zone is formed.
In this case, there is more shear deformation compared with that in flow
pattern A. The extrusion has nonuniform properties compared with that
in flow pattern A.
Flow pattern C is obtained with billets having inhomogeneous material properties or with a nonuniform temperature distribution in the billet. Materials undergo more severe shear deformation at the container
wall and also form a more extended dead-metal zone.
The properties of the extruded aluminum shapes are affected greatly
by the way in which the metal flows during extrusion. The metal flow is
influenced by many factors:
·
·
·
·
·
·
·
·
·
Type of extrusion, direct or indirect
Press capacity and size and shape of container
Frictional effects at the die or both container and die
Type, layout, and design of die
The length of billet and type of alloy
The temperature of the billet and container
The extrusion ratio
Die and tooling temperature
Speed of extrusion
Type, layout, and design of the die might change the mechanical
working of the billet material during extrusion. Hollow dies perform
8.
8 / Aluminum Extrusion Technology
much more mechanical work on the material than simple-shape solid
dies do.
A dead-metal zone builds up in the corners of the die, and the material
shears along this face. The material may continue to extrude over this
generated zone, which acts like a conical die surface. The surface and
subsurface defects are likely to occur on the extruded product if the sufficient amount of butt is not kept. Typical etched cross section of a 7075
alloy butt remaining after extrusion is shown in Fig. 8(a). Figure 8(b)
shows schematically two clear zones. Zone 1 shows the flowing metal
through the rigid conical zone 2, which is defined to be a dead-metal
zone. The darker patches carry oxides and other inclusions into the extruded section, leading to extrusion defects.
The dead-metal zone semiangle may be represented in the functional
form:
α = f(ER, σ, m, m′)
(Eq 1)
where ER is the extrusion ratio, which is defined by the ratio of container bore area and the total cross-sectional area of extrusion, σ is the
flow stress, m is the friction factor between billet and container interface, and m′ is the friction factor between flowing metal and die-bearing
interface.
Under the same friction condition at the billet-container interface for
the same alloy billet, the dead-metal zone semiangle (α) varies with the
extrusion ratio, ER, as shown in Fig. 9. As the extrusion ratio increases,
α increases, and as α increases, the length of shear line decreases. In
Fig. 9, ER1 is the extrusion ratio for the bigger opening die, whereas
ER2 is the extrusion ratio of the smaller opening die, and α2 is the
semidead-metal zone angle corresponding to ER2.
Butt Thickness. According to industry practice, standard butt thickness for direct extrusion is kept to 10 to 15% of the billet length. Butt
thickness may be a function of the dead-metal zone, which is also a
function of the extrusion ratio, type of die, billet temperature, billetcontainer friction condition, and flow stress of the billet material. Figure 10 shows the relationship between butt thickness and the deadmetal zone conical surface. Stopping extrusion at the safe margin zone
prevents oxide and other metallic or nonmetallic inclusions from flowing into the extrusion. It is always recommended to continue research
on macroetching of the longitudinal section of the butt to gain a better
understanding of the following aspects:
•
•
Change of the dead-metal zone conical angle with the change of extrusion variables
Change of the dead-metal zone with the change of die opening
(number of holes) and types of dies (solid and hollow)
9.
(a)
Shear line
2
α
X
X
1
(b)
Fig. 8
Longitudinal cross section of butt after extrusion. (a) Typical etched
cross section of a 7075 butt. (b) Schematic diagram of butt cross section
showing dead zone
10.
10 / Aluminum Extrusion Technology
Fig. 9
Relationship between extrusion ratio and semidead-metal zone angle
Fig. 10
•
•
Relationship between dead zone and butt thickness
Determination of the optimum butt thickness for a set of extrusion
and die variables
Metal flow and formation of the dead-metal zone in case of indirect
extrusion
This is more important for harder alloy extrusion, especially in the aircraft industry. The press should be stopped within the safe margin zone
as shown in Fig. 10.
Plastic Strain and Strain Rate
In order to investigate metal flow quantitatively, it is necessary to define the strain (deformation) and strain rate (deformation rate). In the
theory of metal forming plasticity, the initial condition cannot be used
11.
Fundamentals of Extrusion / 11
as a frame of reference; therefore, the change in length must be related
to instantaneous length. The natural or effective strain is defined by:
d ε = dl
l
l
ε = ∫ dl = ln l
l
l0
l0
(Eq 2)
where, l0 is the initial length, and l is the final length.
The natural strain, ε, obtained by integration is thus a logarithmic
function and is often referred to as the logarithmic strain. The strain in
metal working is given as the fractional cross-sectional area. The volume constancy relation is given by:
Al = A0l0
(Eq 3)
Now, the natural strain is given by:
– = ln l = ln A0
ε
A
l0
(Eq 4)
where A0 is the original area, and A is the final area.
Therefore, the effective strain is defined in the case of extrusion as:
– = 2 ln DC = 2 ln ER
ε
DE
(Eq 5)
where DC is the inside diameter of the container and DE is the equivalent
diameter of the extruded rod, and ER is the extrusion ratio.
In determining the strain rate, the complex flow pattern in the deformation zone creates a problem. The material undergoes a rapid acceleration as its passes through the deformation zone, and therefore, a mean
strain rate has to be estimated for determining the flow stress. The deformation zone is assumed to be conical for simplicity as shown in Fig. 11.
From the geometry, the length of deformation zone is given by:
L=
( DC − DE)
2 tan α
(Eq 6)
where DC is the bore of the container, DE is the diameter of the extruded
rod, and α is the dead-metal zone semiangle.
Equivalent rod diameter for the same extrusion ratio can also be determined. The extrusion ratio of a single-hole die is defined by:
ER = AC
AE
(Eq 7)
12.
12 / Aluminum Extrusion Technology
Fig. 11
Billet geometry inside the container
where AC is the area of the container bore, and AE is the final area of the
extruded rod. Therefore, the equivalent diameter of the extruded rod is
given by:
DE =
DC
ER
(Eq 8)
The mean effective strain rate is given by (Ref 10 and 11):
2
⋅
ε = 6V DC tan α 2 ln DC
3
3
DE
( DC − DE )
(Eq 9)
where V is the average ram speed, DC is the container bore, DE is the diameter of the extruded rod, and α is the dead-metal zone semiangle.
Friction Models
Fundamentals of tribology (friction, lubrication, and wear) are essential in dealing with the field of metal-working processes. During the extrusion of aluminum, the tribology of the die/material interface has a
considerable influence on the accuracy of the shape and surface quality
of the extrusion. In this section, friction modeling of the extrusion process is discussed.
Friction components are totally dependent on the type of extrusions
used, such as direct or indirect. Figure 12 shows the friction-force components in direct extrusion, and similarly, Fig. 13 shows the friction
components in the indirect process using the most common flat-face dies.
From the flow pattern in indirect extrusion using a flat-face die, it is
revealed that a dead-metal zone exists with a much higher angle compared with that in direct extrusion. For the same size extrusion, αi > αd.
Thin butt may be allowed in indirect process. The metal flow in the indirect
13.
Fundamentals of Extrusion / 13
process using a flat-face die may be very similar to the flow with lubricated direct extrusion process.
Friction is the resistance to relative motion that is experienced whenever two solids are in contact with each other. The force necessary to
overcome the resistance, which is directed in the direction opposite to
the relative motion, is the friction force. The Amontons-Coulomb
model (Ref 12) gives the friction force as:
Ff = µN
(Eq 10)
where µ is the coefficient of friction, N is the normal force, and Ff is the
friction force. The model holds fairly well where contacts are relatively
lightly loaded, and the surfaces contact only at occasional asperity
peaks. This model is of questionable value in bulk deformation processes, such as extrusion, where the contact is more intimate and the
pressures are significantly higher.
Billet-Container Interface. The real area of contact increases with
contact pressure as shown in Fig. 14. According to Bowden and Tabor
Fig. 12
Friction components in direct extrusion
Fig. 13
Friction components in indirect extrusion
14.
14 / Aluminum Extrusion Technology
(Ref 13), the friction force using adhesion theory is directly proportional to the real area of contact. In the case of direct extrusion (where
contact pressures are very high), the real area of contact, AR, gradually
becomes equal to the apparent area of contact, AA, as the billet upsets in
the container.
Important considerations in the direct extrusion process are the friction forces developed between the billet and the container and interface
friction between the flowing metal and the dead-metal zone conical interface. In the direct extrusion process, the large pressure developed demands that the billet be supported by the container wall. From a practical point of view, there are two types of friction conditions:
•
•
Billet-container friction is arrested (sticking friction)
Lubricated interface flow is ensured (sliding friction)
In aluminum extrusion, the friction condition at the billet-container
interface is considered to be sticking friction as the skin of the billet is
being separated in the container wall. Schey (Ref 14) provides a useful
review of using the friction factor, m, in metal-forming operations
where the contact pressure is very high. The friction factor model,
sometimes referred to as a stiction model, is:
Ff = mkAR
(Eq 11)
where m is the friction factor, k is the material shear strength, AR is the
real area of contact (which, for this model, equals the total area of contact),
and Ff is the friction force. In the case of sticking friction, m = 1, while
for thick film lubrication conditions, m approaches zero. Therefore, the
frictional stress, τf, is given by:
τf = k =
–
σ
(Eq 12)
3
where k is equal to σ/ 3 according to Von Mises yield criteria, and σ is
the flow stress of the material.
Fig. 14
Friction model in direct extrusion process. (a) AR < AA. (b) AR = AA, p = σ
15.
Fundamentals of Extrusion / 15
Dead-Metal Zone-Flowing Metal Interface. The dead-metal zone
shown in Fig. 12 occurs when a material is extruded through square dies
(i.e., the bearing surface is perpendicular to the face of the die). In such
geometry, the material in the corners no longer takes part in the flow but
adheres to the die face, forming a conical die-like channel through
which the billet passes in a still-converging kind of flow. Friction between the dead-metal zone and the flowing material is no more than the
shear stress of the material. The friction stress is also given by Eq 12
with friction factor equal to unity.
Die-Material Interface. Based on the observation of the die surface
after several extrusion cycles, it is understood that friction in the die can
vary in a complicated way when metal is flowing through the die opening. It has been observed that an adhesive layer on the die develops due
to the strong adhesion of materials such as aluminum with the dies, typically constructed from tool steels. It is also understood that surface
treatments (such as nitriding or thin hard coatings) that result in harder
die bearing can reduce the amount of adhered aluminum on the die bearing. Research is continuing on die bearing treatments for wear resistance.
A friction model developed by Abtahi (Ref 15) is based on measured
slipping and sticking lengths using a split die. This model shows almost
constant friction in the sticking region, whereas in the slipping region,
friction is changing with the die angle.
Proposed Model. In a recent study, Saha (Ref 16) suggested a friction model at the die-material interface. Figure 15 is a schematic of the
bearing surface based on the morphology of aluminum buildup on the
die bearing, which is normal to the extrusion direction. Figure 15 also
shows the sticking and slipping zones of the die that are used to develop
a friction model at the die-material interface. Figure 15(a) shows partial
sticking and slipping zones, and Fig. 15(b) shows a completely adhered
surface. After several press cycles, a completely adhered surface is developed on the die face.
During extrusion, the normal pressure on the bearing surface of the
die is very high. This pressure is assumed to be equal to the extrusion
pressure, which is equal to or higher than the flow stress of the material.
Based on the definition of the friction factor, the friction force Ff on the
die is given by:
Ff = m1 k AR1 + m2 k AR2
(Eq 13)
where a 1 subscript denotes a sticking zone, a 2 subscript denotes a sliding zone, m is the friction factor, AR is the real area of contact, and k is
the material shear strength. The friction stress is given by:
τ f = k AR1 + m2 k AR 2
AA
AA
(Eq 14)
16.
16 / Aluminum Extrusion Technology
Fig. 15
Schematic of the morphology of the die bearing surface
where AA is the apparent area of contact for the entire bearing surface,
and m1 has been set equal to unity to reflect sticking friction.
In the case of complete adhesion (sticking friction) on the die bearing,
m2 = 1; accordingly, the frictional stress will be changed to:
–
A + AR2
σ
τ f = k R1
=k=
AA
3
(Eq 15)
Extrusion Pressure
The parameter that determines whether extrusion will proceed or
whether a sticker will result is the magnitude of the maximum pressure
that must be within the extrusion press capacity. The factors that influence successful extrusion are as follows:
•
•
•
•
•
•
•
Extrusion temperature
Temperature of container, die, and associated tooling
Extrusion pressure
Extrusion ratio
Extrusion speed
Billet length
Chemistry of the alloy
In the direct extrusion process, pressure reaches a maximum at the
point of breakout at the die. A typical pressure curve is shown in Fig. 2.
The difference between the maximum and minimum pressures can be
attributed to the force required in moving the billet through the container against the frictional force. The actual pressure exerted on the
17.
Fundamentals of Extrusion / 17
ram is the total pressure. The total extrusion pressure required for a particular extrusion ratio is given by:
PT = PD + PF + PR
(Eq 16)
where PD is the pressure required for the plastic deformation of the material, which is given in the functional form as:
PD =f (σ, ε)
(Eq 17)
where the flow stress, σ, is defined by:
⋅
–
σ = f (ε , ε , T )
(Eq 18)
strain and strain rate are defined by:
– = ln AC
ε
AE
(Eq 19)
⋅
ε
– = d–
ε
dt
(Eq 20)
and T is the temperature of the material.
PF is the pressure required to overcome the surface friction at the container wall friction, dead-metal zone friction, and die bearing friction,
which is given in the functional form
PF = f (pr, m, m′, m″, D, L, L′)
(Eq 21)
where pr is the radial pressure, m is the friction factor between the billet
and container wall, m′ is the friction factor at the dead-metal zone/flowing
metal interface, m″ is the friction factor between extruded material and
die bearing, D is the billet diameter, L is the length of the billet, and L′ is
the die bearing length of a solid die.
PR is the pressure to overcome redundant or internal deformation
work, which is given in the functional form
PR = f (σ, α)
(Eq 22)
where α is the semidead-metal zone angle as a function of the extrusion
ratio.
Dieter (Ref 2) has given a nice explanation of the redundant work. Elements at the center of the billet undergo essentially pure elongation in
the extruded rod, which corresponds to the change in cross section from
billet to extrusion. The elements shown in Fig. 16, near the container
wall, undergo extensive shear deformation due to billet-container interface
18.
18 / Aluminum Extrusion Technology
friction. The elements at the dead-metal zone interface also undergo extensive shear deformation. The shear deformation, which occurs over
much of the cross section of the extruded rod, requires an expenditure of
energy. This energy expenditure, which is not related to the change in
dimensions from the billet to the extrusion, is called redundant work, as
shown in Fig. 16. The redundant work is mainly responsible for the
large difference between the actual extrusion pressure and the calculated pressure on the basis of uniform plastic deformation.
For a given size of billet extruded under a particular set of conditions,
there will be an upper limit to the extrusion ratio that can be obtained
with a press of a given capacity. The temperature of extrusion plays the
most important role in getting a properly extruded product, and extrusion speed are also important factors. An increase in the length of the
billet, however, results in raising the pressure required for extrusion.
This increase in pressure is due to the frictional resistance between the
billet and the container wall, which is greater for the longer billet.
Normally, the maximum length of the billet is four times its diameter.
In extrusion of metals, there are certain interrelations between extrusion pressures, extrusion temperatures, extrusion ratios, and extrusion
speeds:
•
•
•
Increase in the temperature of the billet reduces the pressure required for extrusion.
The higher the extrusion ratio, the higher the extrusion pressure.
The greater the billet length, the higher the extrusion pressure.
Fig. 16
Redundant work
19.
Fundamentals of Extrusion / 19
•
Billet temperature remains within extrusion range; extrusion pressure remains fairly unaffected when extrusion speed is increased
within normal limits.
Analysis of Extrusion Pressure
Slab Method. In this section, the average extrusion pressure during
direct extrusion of aluminum is calculated by using the slab method.
Thomsen et al. (Ref 7) have shown an analysis by using a uniform energy method, slab analysis, and slip-line field theory. Altan et al. (Ref
17) have performed a slab method analysis to determine the extrusion
pressure. The following considerations were used in making the analysis:
•
•
•
•
Extrusion using a cylindrical billet through a flat die
Extrusion shape equivalent to a rod of diameter DE
Frictional shear stress at the dead-metal/flowing metal interface
Frictional shear stress at the billet-container interface
Consider the static equilibrium of the forces acting on the shaded element within the dead-metal zone area as shown in Fig. 17. The stresses
acting on this slab are shown in Fig. 18(b). The equilibrium equation is
given by:
2
2
π ( D + dD)
+ pz πD + pr π D ds sin α
4
4
+ τ f πD ds cos α = 0
− ( pz + dpz)
(Eq 23)
where τf is the frictional stress at the dead-metal zone/flowing material
interface, pr is the radial pressure and α is the semidead-metal zone angle.
This equation can be simplified by using the following geometric relationship among dz, dD, and ds:
ds sin α = dz tan α =
ds cosα = dz =
dD
2
dD
2 tan α
(Eq 24)
(Eq 25)
From the yield criterion,
pr = pz + σ
(Eq 26)
where pr is the radial pressure, pz is the pressure in the Z direction and σ
is the flow stress of the material.
20.
20 / Aluminum Extrusion Technology
Combining Eq 23, 24, 25, and 26, substituting τf from Eq 12, and neglecting the higher order differentials, the equilibrium equation is obtained in the integral form:
dpz
2dD
– (1 + cot α ) = D
σ
3
(Eq 27)
Assuming the flow stress remains constant, the integration of the equation yields:
pz
2
= ln D C
cot α
–
)
σ (1 +
3
(Eq 28)
where C is the integration constant.
Fig. 17
Fig. 18
Extrusion through a square die with dead-metal zone and equivalent rod diameter
State of stress for the extrusion shown in Fig. 17. (a) Freebody diagram of element inside the container wall. (b) Freebody diagram of
element under the dead-metal zone. (c) Geometric relationship among dz, dD,
and ds
21.
Fundamentals of Extrusion / 21
Substituting the boundary conditions at D = DE, pz = 0, C will be determined by:
C=
1
(Eq 29)
2
DE
where DE, the equivalent diameter of extruded rod, could be calculated
by using Eq 8.
Substituting the value of constant, C, in Eq 28 and simplifying, the average extrusion pressure is given by:
–
pave, z=0 = 2σ (1 + cot α ) ln DC
DE
3
(Eq 30)
where DC is the equivalent diameter of the billet (container bore diameter) filled in the container after upsetting.
Billet-Container Interface Friction. Billet-container interface friction must be included to determine the total pressure required for extrusion from a round-shaped billet to an equivalent rod. Considering the
shaded element in the cylindrical portion (Fig. 17), the equation expressing static equilibrium in the Z direction is given by:
2
[( pz + dpz ) − pz]πDC = π DCτ f dz
4
(Eq 31)
where, τf is the friction force at the billet-container interface, DC is the
diameter of the container bore. Equation 31 may be written in the integral form:
dpz
4
τ f = DC dz
(Eq 32)
Integrating Eq 32 and putting the boundary condition: at Z = 0, pz =
pave, z=0, the average extrusion pressure may be written as:
pz =
4τf Z
+ pave, z =0
DC
(Eq 33)
Now substituting pave, z=0 from Eq 30 and τf from Eq 12, the average
extrusion pressure may be written as:
–
–
pave = 2σ (1 + cot α ) ln DC + 4σZ
DE
3
3 DC
(Eq 34)
22.
22 / Aluminum Extrusion Technology
Avitzur (Ref 18) used an upper-bound method to derive an equation to
predict extrusion load.
Extrusion Force
The force required for extrusion depends on the flow stress of the billet material, the extrusion ratio, the friction condition at the billet container interface, the friction condition at the die material interface, and
the other process variables, such as initial billet temperature and the
speed of extrusion. The required extrusion force, Fr, is given by:
Fr = PTAC
(Eq 35)
where PT is the extrusion pressure, and AC is the area of the container
bore.
The force term is essential in determining the capacity of the extrusion press. The external force given by the extrusion press will determine the press capacity. For successful extrusion, the force balance has
to be satisfied as follows:
Fp > Fr
where Fp is the force applied by the press, and Fr is the force required for
extrusion. Force (compression power) applied by the press is given by:
Fp = pA1 + p(2A2)
(Eq 36)
where A1 is the area of the main cylinder, A2 is the area of each side cylinder, and p is the applied hydraulic pressure to the cylinders as shown
in Fig. 19.
Specific pressure (inner pressure in the container liner) as shown in
Fig. 20 is given by:
Fp
Ps = A
C
(Eq 37)
Effect of Principal Variables on Extrusion
Extrusion can become impossible or can yield an unsatisfactory product when the load required exceeds the capacity of the press available or
when the temperature of the extrusion exceeds the solidus temperature
of the alloy. Knowledge of the initial billet temperature, the strain-rate,
flow stress of the working material, and the extrusion ratio are required
if correct and economical use is to be made of expensive extrusion facilities.
23.
Fundamentals of Extrusion / 23
Fig. 19
Schematic of direct extrusion press
Fig. 20
Specific applied pressure
Principal Variables
The principal variables (Fig. 21) that influence the force required to
cause extrusion and the quality of material exiting from the die are as
follows:
•
•
•
•
Extrusion ratio
Working temperature
Speed of deformation
Alloy flow stress
Extrusion Ratio. The extrusion ratio (ER) of a multihole die is defined by:
ER = AC
n( AE)
(Eq 38)
24.
24 / Aluminum Extrusion Technology
where n is the number of symmetrical holes, AC is the area of container,
and AE is the area of extrusion. The extrusion ratio of a shape is a clear
indication of the amount of mechanical working that will occur as the
shape is extruded.
The effective strain is a function of the extrusion ratio, and finally, extrusion pressure required to extrude is a function of strain. When the extrusion ratio of a profile is low, the amount of plastic strain is also low.
As a result, the amount of work done during extrusion will be less. In
aluminum extruded with a low extrusion ratio, the structure will be similar to that of as-cast (coarse grain) aluminum. This structure will be
mechanically weak, and as a result, shapes with an extrusion ratio of
less than 10 to 1 may not be guaranteed to meet the mechanical and
physical properties specifications of the material.
When the extrusion ratio is high, the situation is just the opposite as
expected. The extrusion pressure required to push the metal through the
die will be higher due to a higher amount of plastic strain. The normal
extrusion ratio range in industry practice for hard alloys is from 10 to 1
to 35 to 1, and for soft alloys, 10 to 1 to 100 to 1. However, these normal
limits should not be considered absolute because the actual shape of the
extrusion affects the results.
Extrusion Temperature. Extrusion is commonly classified as a
hot-working process. Hot working is defined as deformation under conditions of temperature and strain-rate such that recovery processes take
place simultaneously with deformation. Extrusion is carried out at elevated temperatures for metals and alloys that do not have sufficient
plasticity range at room temperature and also to reduce the forces required for extrusion.
Temperature is one of the most important parameters in extrusion.
The flow stress is reduced if the temperature is increased and deformation is, therefore, easier, but at the same time, the maximum extrusion
speed is reduced because localized temperature can lead to the incipient
melting temperature. The changes during extrusion depend on the billet
Fig. 21
Principal extrusion variables
25.
Fundamentals of Extrusion / 25
temperature, the heat transfer from the billet to the container, and the
heat developed by deformation and friction. In actual aluminum extrusion practice, very complex thermal changes commence as soon as the
hot billet is loaded into the usually preheated container, and extrusion is
started.
Temperature rise and temperature distribution during extrusion have
been investigated by many researchers (Ref 10, 11, 16, and 19–23). In
the next chapter, thermal considerations in aluminum extrusion, including isothermal extrusion, will be discussed in more detail.
Extrusion Speed. The response of a metal to extrusion processes can
be influenced by the speed of deformation. Increasing the ram speed
produces an increase in the extrusion pressure. The temperature developed in extrusion increases with increasing ram speed. This increase is
due to the fact that the strain rate is directly proportional to the ram
speed, and the magnitude of the generated heat is proportional to the
strain rate. The slower the ram speed is, the more time will be available
for the generated heat to flow. The heat conduction is more pronounced
with aluminum because of its higher conductivity.
Relationship Between Ram Speed and Extrusion Speed (Ref 24). This
section explains how to calculate the extrusion speed in terms of ram
speed by using simple mathematical relations. The extrusion speed
could be calculated for any extrusion die by using volume constancy relation, which means that the volume metal in the container becomes
equal to the volume of extrusion coming out of the die because there is
no loss of metal during extrusion.
From volume constancy as shown in Fig. 21, it is given by:
VR AC = VE AE
(Eq 39)
where VR is the ram speed, AC is the area of the container bore, VE is the
extrusion speed, and AE is the area of the extruded shape.
If it is a multi-hole die, the relationship will be changed according to
the number of holes in the die, which is given by:
VR AC = VE(n AE)
(Eq 40)
where n is the number of symmetrical holes.
The extrusion speed is given by:
VE = VR
AC
n( AE)
(Eq 41)
The extrusion speed could also be written as:
VE = VR ER
(Eq 42)
26.
26 / Aluminum Extrusion Technology
where ER is defined by:
AC
n( AE)
Material Flow Stress. A true stress-strain curve is frequently called a
flow curve because it gives the stress required to cause the metal to flow
plastically to any given strain. The flow stress, σ, is important because in
plastic deformation process, the forming load or stress is a function of
part geometry, friction, and the flow stress of the deforming material.
The flow stress of the material is influenced by the following factors:
•
•
Chemistry and the metallurgical structure of the material
Temperature of deformation, the amount of deformation or strain, ε,
⋅
and the rate of deformation or strain-rate, ε
Therefore, the flow stress can be written in a functional form:
⋅
–
σ = f (–, – , T )
ε ε
(Eq 43)
Because the flow stress for hot-working metal is quite markedly affected by the speed of deformation, there are no specific methods for
measuring the flow stress during the hot-working process. The flow
stress of the billet material depends on both strain rate and temperature.
The decrease in flow stress with increasing temperature and the increase at higher strain rate have been measured in several studies. The
flow stress of metal for the actual working conditions is determined experimentally. The methods most commonly used for obtaining flow
stress are tensile, uniform compression, and torsion tests.
The effect of temperature measured in the experiments to determine
the flow stress can be directly applied to extrusion. Laue and Stenger
(Ref 3) have given a complete review of experimental values of flow
stress by many authors. The relationship between flow stress and strain
rate has been used in numerical analysis to determine the influence of
plastic strain and strain rate on temperature in aluminum 6063 extrusion
(Ref 21). Because the accuracy of this type of analysis is very much dependent on the flow stress of material, this relationship fits very well for
determining the flow stress of different aluminum alloys for the most
common working temperature.
The relationship is given by (Ref 3):
σ = σ0
⋅ m*
ε
⋅
ε0
(Eq 44)
27.
Fundamentals of Extrusion / 27
Fig. 22
Effect of principal variables on extrusion
⋅
where, σ0 is the known flow stress at a known strain-rate ε 0 , and simi⋅
larly, σ is the flow stress at the strain rate ε. For example, a typical value
of the exponent, m*, at 932 °F (500 °C) for AlMgSi1 alloy is 0.125.
As a rule, for the flow stress of the alloy being extruded, the lower the
extruded rate, the greater the friction between the billet and the container wall because of higher critical shear stress, and the longer the
time required to overcome friction and start the extrusion. Primarily,
this is the result of the increased flow stress of the material, and the hard
alloy requires maximum pressure for extrusion. The extrusion of hard
alloy is even more difficult because of poor surface characteristics,
which demand the lowest possible billet temperatures.
A summary of the effects of different factors on extrusion and their interrelationship are shown in Fig. 22 as a closed-loop chain.
References
1. S. Kalpakjian, Manufacturing Engineering and Technology, 2nd
ed., Addison-Wesley Publishing Company, 1992
2. G.E. Dieter, Mechanical Metallurgy, McGraw-Hill, Inc., 1961
3. K. Laue, and H. Stenger, Extrusion, American Society for Metals,
1981
4. W.A. Backofen, Deformation Processing, Addison-Wesley Publishing Company, 1972
5. G.W. Rowe, Principle of Industrial Metalworking Processes, Edward Arnold Publisher, London, 1977
6. W. Johnson and P.B. Mellor, Engineering Plasticity, Van Nostrand
Reinhold Company, London, 1975
7. E.G. Thomsen, C.T. Yang, and S. Kobayashi, Mechanics of Plastic
Deformation in Metal Processing, The Macmillan Company, 1965
8. E.C. Pearson and R.N. Parkins, The Extrusion of Metals, 2nd ed.,
Chapman and Hall Ltd., London, 1960
28.
28 / Aluminum Extrusion Technology
9. H. Valberg, A Modified Classification System for Metal Flow
Adapted to Unlubricated Hot Extrusion of Aluminum and Aluminum Alloys, Proc. Sixth International Aluminum Extrusion Technology Seminar, Aluminum Extruders Council and The Aluminum
Association, Inc., May 1996
10. A.F. Castle and T. Sheppard, Hot Working Theory Applied to Extrusion of Some Aluminum Alloys, Met Technol., Vol 3 (No. 10),
1976
11. A.F. Castle, Temperature Control in Aluminum Extrusion, Proc.
Fifth International Aluminum Extrusion Technology Seminar, Aluminum Extruders Council and the Aluminum Associations,
Inc.,1992
12. G. Amontons, Hist. Acad. R. Soc., Paris, 1699
13. F.P. Bowden and D. Tabor, “The Friction and Lubrication of Solids,
Part II,” Oxford University Press, 1964
14. J.A. Schey, Tribology in Metalworking, American Society for
Metals, 1983
15. S. Abtahi, Interface Mechanisms on the Bearing Surface in Extrusion, Proc. Sixth International Aluminum Extrusion Technology
Seminar, May 1996
16. P.K. Saha, Thermodynamics and Tribology in Aluminum Extrusion, Wear, Vol 218, 1998
17. T. Altan, Soo-lk. Oh, and L. Harold Gegel, Metal Forming: Fundamentals and Applications, American Society for Metals, 1983
18. B. Avitzur, Metal Forming: Process and Analysis, McGraw-Hill
Book Company, 1968
19. T. Altan and S. Kobayashi, A Numerical Method for Estimating the
Temperature Distribution in Extrusion Through Conical Dies, J.
Eng. Ind. (Trans. ASME), 1968
20. Y. Tashiro, H.Yamasaki, and N. Ohneda, Extrusion Conditions and
Metal Flow To Minimize Both Distortion and Variance of CrossSectional Shape, Proc. Fifth International Aluminum Extrusion
Technology Seminar, 1992
21. P.K. Saha, Temperature Distribution in Extrusion, M.S. thesis, University of Calcutta, India, 1977
22. P.K. Saha, and R.K. Ghosh, Temperature Distribution During Hot
Extrusion of Aluminum—Theoretical Evaluation, Indian J.
Technol., Vol 17, 1979
23. P.K. Saha, Influence of Plastic Strain and Strain Rate on Temperature Rise in Aluminum Extrusion, Proc. Sixth International Aluminum Extrusion Technology Seminar, Vol 2, Aluminum Extruders
Council and the Aluminum Associations, Inc., May 1996
24. P.K. Saha, Factors Affecting Speed and Pressure in 6063 Aluminum Extrusion, Proc. Aluminum 2000—3rd World Congress on
Aluminum, 1997 (Cyprus), Interall Publications
Views
Actions
Embeds 0
Report content